advertisement

Solid State Chemistry CHM4627 Prerequisite Courses : Inorganic Chemistry, CHM3610, and Physical Chemistry, CHM4410C, or permission of the instructor. Prerequisite Knowledge: Geometry and Trigonometry – Cosine, sine, tangent, triangle rules General Chemistry I - periodic table, ions and ionic compounds, stoichiometry, formula weights, interconverting masses and moles, thermochemistry, enthalpy, wave behavior of matter, quantum mechanics and atomic orbitals, representations of orbitals (s,p,d,f), electron spin and Pauli exclusion principle, electron configurations, effective nuclear charge, sizes of atoms and ions (trends), electron affinity, electronegativity, group trends, Lewis symbols, ionic bonding and energetics, covalent bonding, molecular geometry and bonding theories, VSEPR, covalent bonding and orbital overlap, molecular orbitals for simple diatomic molecules. General Chemistry II – Phase changes, phase diagrams, structures of solids, unit cells, close packing of spheres, bonding in solids (molecular, covalent network, ionic, metallic), chemical kinetics, Le Chatelier’s Principle, classical thermodynamics, entropy, Gibbs Free energy, oxidation states, balancing oxidation-reduction reactions, crystal field theory, electron configuration in complexes. Solid State Chemistry The solid state chemistry course is an in-depth examination of the principles and concepts underlying the synthesis, structure, bonding, reactivity, and physical properties of solid state materials. Three hours lecture. Tentative Topics: •Introduction to Crystal Structures •Physical Methods for Characterizing Solids •Synthesis Methods •Bonding and Electronic Properties •Defects and Non-Stoichiometry •Microporous and mesoporous solids •Optical Properties of Solids •Magnetic and Dielectric Properties •Superconductivity •Nanostructures and Low Dimensional properties 1 Solid state chemistry - the study of synthesis, structure, bonding, reactivity, and physical properties of solids. •interdisciplinary overlap with condensed matter physics, mineralogy, crystallography, metallurgy, ceramics, and materials science. Brief history and notable contributions from solid state chemistry •X-ray crystallography in the early 1900’s by William L Bragg •Zeolite and platinum-based catalysts for petroleum processing in the 1950’s •High-purity silicon, a core component of microelectronic devices in the 1960’s •Microwave dielectrics (wireless communications) in the 1970’s •‘High temperature’ superconductivity in the 1980’s •Giant and colossal magnetoresistive (CMR) materials in the 1990’s •Nano-, energy storage and generation, and functional materials in the 2000’s It’s a portable phone! Solids Solid State Chemistry, a subdiscipline of Chemistry, primarily involves the study of extended solids. •Except for helium*, all substances form a solid if sufficiently cooled at 1 atm. •The vast majority of solids form one or more crystalline phases – where the atoms, molecules, or ions form a regular repeating array (unit cell). •The primary focus will be on the structures of metals, ionic solids, and extended covalent structures, where extended bonding arrangements dominate. •The properties of solids are related to its structure and bonding. •In order to understand or modify the properties of a solid, we need to know the structure of the material. •Crystal structures are usually determined by the technique of X-ray crystallography. •Structures of many inorganic compounds may be initially described in terms of simple packing of spheres. 2 Close-Packing Square array of circles Close-packed array of circles Considering the packing of spheres in only 2-dimensions, how efficiently do the spheres pack for the square array compared to the close packed array? 3 Layer A Layer B ccp cubic close packed hcp hexagonal close packed 4 Layer B (dark lines) CCP HCP In ionic crystals, ions pack themselves so as to maximize the attractions and minimize repulsions between the ions. •A more efficient packing improves these interactions. •Placing a sphere in the crevice or depression between two others gives improved packing efficiency. hexagonal close packed (hcp) ABABAB Space Group: P63/mmc cubic close packed (ccp) ABCABC Space Group: Fm3m 5 Face centered cubic (fcc) has cubic symmetry. Atom is in contact with three atoms above in layer A, six around it in layer C, and three atoms in layer B. A ccp structure has a fcc unit cell. 6 Coordination Number hcp ccp The coordination number of each atom is 12. Primitive Cubic 7 Body Centered Cubic (bcc) How many atoms in the unit cell of the following? Primitive (P) Body Centered (I) Face-Centered (A, B, C) All Face-Centered (F) 8 8(1/8) + 6(1/2) = 4 atoms per unit cell Spheres are in contact along the face diagonal, thus l = d√2. The fraction of space occupied by spheres is: V spheres V unitcell 4 3 3 ( d / 2 ) 4 0 . 74 (d 2 )3 The density expression is: Density( g / cm3 ) Packing Efficiency: ratio of space occupied by spheres to that of the unit cell It is the most efficient (tied with hcp) packing scheme. number of formula units ( FW / 6.022 10 23 (in g/atom)) Vunitcell (cm 3 ) Occurrence of packing types assumed by elements The majority of the elements crystallize in hcp, bcc, or ccp(fcc). Polonium adopts a simple cubic structure Other sequences include ABAC (La, Pr, Nd, Am), and ABACACBCB (Sm). Actinides are more complex. 9 Pressure-temperature phase diagram for iron 10 Symmetry Symmetry is useful when it comes to describing the shapes of both individual molecules and regular repeating structures. Point symmetry - is the symmetry possessed by a single object that describes the repetition of identical parts of the object Symmetry operations – are actions such as rotating an object or molecule (^) Symmetry elements – are the rotational axes, mirror planes, etc., possessed by objects Schoenflies- useful in describing the point symmetry of individual molecules (spectroscopists) Hermann-Mauguin – can describe the point symmetry of individual molecules, and also the relationship of different atoms to one another in space (space symmetry) Hermann-Mauguin: Axes of Symmetry: 2, 3, 4, 6 Proper axes of rotation (Cn) Rotation with respect to a line (axis of symmetry) which molecules rotate. •Cn is a rotation of (360/n)°, where n is the order of the axis. •C2 = 180° rotation, C3 = 120° rotation, C4 = 90° rotation, C5 = 72° rotation, C6 = 60° rotation… •Each rotation brings you to the indistinguishable state for original. However, rotation by 90° about the same axis does not give back the identical molecule. Therefore H2O does NOT possess a C4 symmetry axis. XeF4 is square planar. It has four different C2 axes. A C4 axis out of the page is called the principle axis because it has the largest n. By convention, the principle axis is in the z-direction 11 Hermann-Mauguin: Planes and Reflection (σ) m Molecules contain mirror planes, the symmetry element is called a mirror plane or plane of symmetry. •σh(horizontal): plane perpendicular to principal axis •σd(dihedral), σv(vertical): plane colinear with principal axis •σv: Vertical, parallel to principal axis •σd: σ parallel to Cn and bisecting two C2' axes Hermann-Mauguin: Inversion, Center of Inversion (i) 1 A center of symmetry: A point at the center of the molecule. (x,y,z) → (-x,-y,-z). Tetrahedrons, triangles, and pentagons don't have a center of inversion symmetry. Ru(CO)6 C 2H 6 12 Hermann-Mauguin: n Rotation-reflection, Improper axis (Sn) •This is a compound operation combining a rotation (Cn) with a reflection through a plane perpendicular to the Cn axis σh.(Cn followed by σh) σCn=Sn (Schoenflies) •It may be viewed as a combination of a rotation (1/n of a rotation) and inversion. (Hermann-Mauguin) Equivalent Symmetry elements in Schoenflies and Hermann-Maguin Systems Schoenflies HermannMauguin S1 ≡ m 2≡m S2 ≡ i 1≡i S3 6 S4 4 S6 3 solid state molecular spectroscopy Hermann-Mauguin inversion axis 1 n 4 13 Symmetry: Individual Molecules to Crystals The molecules are related in space by a symmetry element they do not possess, this is the site symmetry. Crystals 14 Lattices and Unit Cells A crystal is a solid in which the constituent atoms, molecules, or ions are packed in a regularly ordered, repeating pattern of ‘building blocks’, extending in all three spatial dimensions. -the ‘building block’ is known as the unit cell. Simplest regular array is a line of evenly spaced objects (one-dimensional). a The line of dots is called the lattice, and each lattice point (dot) must have identical surroundings. The choice of unit cell is arbitrary. a Lattice + basis + = crystal structure = Lattice points are associated to a basis + lattice = basis CRYSTAL STRUCTURE = lattice + basis (atoms or ions) 15 Crystal Lattices Space lattice a pattern of points that describes the arrangement of ions, atoms, or molecules in a crystal lattice. Unit Cell the smallest, convenient microscopic fraction of a space lattice that: 1. When moved a distance equal to its own dimensions (in various directions) generates the entire space lattice. 2. reflects as closely as possible the geometric shape or symmetry of the macroscopic crystal. Although crystals exist as three dimensional forms, first consider 2D. A crystal contains approximately Avogadro’s number of atoms, ions, or molecules. The points in a lattice extend pseudo infinitely. How does one describe the entire space lattice in terms of a single unit cell? What kinds of shapes should be considered? Square 2d array Select a unit cell based on, 1. Symmetry of the unit cell should be identical with symmetry of the lattice 2. Unit cell and crystal class (triclinic…) are related 3. The smallest possible cell should be chosen 16 Rectangular 2d array Centered cell (C) – have a lattice point at each corner and one totally enclosed in the cell. Primitive cell (P) – have a lattice point at each corner and contain one lattice point. 17 Five Types of Planar 2-D Lattices Translational Symmetry Elements – Glide Plane and Screw Axis Glide plane – combination of translation with reflection. z x a y + , Glide plane + Glide direction + a/2 Comma indicates that some molecules when reflected through a plane of symmetry are enantiomorphic, meaning the molecule is not superimposable on its mirror image. 18 Translational symmetry elements: Glide plane 1. Reflection at a mirror plane 2. Translation by t/2 (glide component) Axial glides a, b, c a/2, b/2, c/2 Diagonal glides n Vector sum of any two a/2, b/2, c/2, e.g. a/2 + b/2 Diamond glide d Vector sum of any two a/4, b/4, c/4, e.g. a/4 + b/4 Screw axis –combination of translation with rotation. –uses the symbol ni, where n is the rotational order of the axis (twofold, threefold, etc.) and the translation distance is given by the ratio i/n. y Example of a 21 screw axis z c x 21 Screw axis + + c/2 19 Rotation axis Screw axis Symmetry elements with respect to an axis Rotation angle q = 360°/ X, X = # of rotations Symbol q 1-fold 2-fold 3-fold 4-fold 6-fold axis: axis: axis: axis: axis: 360° 180° 120° 90° 60° 1 2 3 4 6 5-fold, 7-fold, 8-fold, 10-fold (…) axes are not possible in 3 dimensional space.* *2011 Nobel Prize in Chemistry, Dan Shechtman "for the discovery of quasicrystals“ notwithstanding 20 http://www.nobelprize.org/nobel_prizes/chemistry/laureates/2011/press.html Three-Dimensional Unit Cells The unit cell of a three-dimensional lattice is a parallelepiped defined by three distances (a, b, c) and three angles (a, b, g). 7 Lattice systems 14 Bravais lattices Different ways to combine 3 non-parallel, non-coplanar axes Compatible with 32 3-D point groups (or crystal classes) Combine 14 Bravais Lattices, 32 translation free 3D point groups, and glide plane and screw axes result in 230 space groups. 21 Seven Lattice systems Seven Crystal Systems or Classes Minimum symmetry requirement Four threefold axes at 109°28’ to each other One fourfold axis or one fourfold improper axis. Any combination of three mutually perpendicular twofold axes or planes of symmetry (H) One sixfold axis or one sixfold improper axis; (R) one threefold axis One twofold axis or one symmetry plane None 22 Miller Indices A lattice plane is a plane which passes through any three points which are not in a straight line. A set of parallel lattice planes is characterized by its Miller indices (hkl). The set of lattice planes (hkl) divides a into h parts, b into k parts, and c into l parts, where a, b, and c are the lengths of the unit-cell sides. Two-dimensional example The indices of a line hk are defined so that the line intercepts a at a/h and b at b/k. 1. Consider the line that is adjacent to the one that passes through the origin. 2. Find the intersections and write these as fractions of the cell edges. 3. Take the reciprocal of the fractions. z y x The indices of a line hkl are defined so that the line intercepts a at a/h, b at b/k, and c at c/l. 1. Consider the plane that is adjacent to the one that passes through the origin. 2. Find the intersections and write these as fractions of the cell edges. 3. Take the reciprocal of the fractions, which give the (hkl) or index of the plane. 23 Intercepts: a, , Intercepts: a, a, Intercepts: a, a, a Reciprocals: a/a, a/, a/ = 1, 0, 0 Reciprocals: a/a, a/a, a/ = 1, 1, 0 Reciprocals: a/a, a/a, a/a = 1, 1, 1 Miller index for this plane: hkl = (1 0 0) Miller index for this plane : hkl = (1 1 0) Miller index for this plane : hkl = (1 1 1) Interplanar Spacing The perpendicular spacing (d spacing) between parallel planes (Miller indices hkl) may be calculated using the following equations. 24 Fractional Coordinates The position of an atom or ion in a unit cell is described by its fractional coordinates. Fractional coordinates (x, y, z) are expressed as fractions of the length of the sides of the unit cell (a, b, c) c (0, 0, 0) (0, 0, 0) b (0.5, 0.5, 0.5) a (0, 0, 0) (0, 0.5, 0.5) (0.5, 0, 0.5) (0, 0, 0) (0.5, 0, 0.5) (0.5, 0.5, 0) Crystalline Solids Ionic •Consider an interaction between a metal with a low ionization energy and a nonmetal with a highly exothermic electron affinity. •Electrons are transferred to produce cations and anions, forming a strong, non-direction electrostatic attraction between the ions. •Ions pack together to maximize the coulombic attraction between oppositely charged ions and minimize the repulsion between ions of the same charge. Covalent •In many structures, the bonding is not completely ionic, but possesses some degree of covalency, where the electrons are shared between the two bonding atoms and not merely transferred from one to the other. Other •In addition to ionic and covalent bonding, other bonding and interactions include metallic bonding and intermolecular forces such as hydrogen bonds, dipole-dipole forces, and London dispersion forces. 25 Ionic Solids (MX) CsCl Other Compounds: CsBr, CsI, TlCl, TlBr, TlI, NH4Cl Rock Salt - NaCl 2x2 supercell Other Compounds (200+): Most alkali halides, all the alkali hydrides, AgF, AgCl, AgBr, MO (M = Mg, Ca, Sr, Ba), MS (M = Mg, Ca, Sr, Ba) 26 Linked Octahedra [MX6] Octahedron Solid Octahedron (polyhedral) Corner-sharing Edge-sharing Two octahedra = M2O11 Two octahedra =M2O10 Face-sharing Two octahedra= M2O9 NaCl showing edge-sharing of octahedra and an enclosed tetrahedral space. 27 Structure Type - Nickel Arsenide (NiAs) Equivalence to the sodium chloride structure in hcp. It can be described as an hcp array of arsenic atoms with nickel atoms occupying the octahedral holes. As is located in the center of a trigonal prism of six nickel atoms. Structure Type – Fluorite (CaF2) The structure can be described as a ccp array of calcium ions, with fluoride ions occupying all the tetrahedral holes. •Note that Ca2+ ions are smaller than F-, so it is not fully described as a ccp array, but this description gives an exact description of the relative positions of the ions. •The larger octahedral holes are unoccupied in this structure, which is important when considering the movement of ions in defect structures. •By drawing cubes of fluoride ions, the structure is now divided into octants with alternate octants occupied by calcium. •In antifluorite, the positions of cation and anions are reversed. 28 Structure Type – Zinc Blende / Sphalerite (ZnS) A ccp array of sulfide ions with zinc ions occupying every other tetrahedral hole in an ordered manner. Compounds adopting this structure include copper halides, Zn, Cd, and Hg sulfides. If all atoms are the same, the structure would be identical to C (diamond). Structure Type – Wurtzite (ZnS) The Wurtzite structure type is composed of an hcp array of sulfide ions with alternate tetrahedral holes occupied by zinc ions. BeO, ZnO, NH4F also adopt this structure type. 29 Structure Type – Cadmium Chloride (CdCl2) Close packing of anions (ccp) with half of the octahedral holes occupied by cations. •The cations occupy all the octahedral holes in every other layer, giving an overall layer structure with 6:3 coordination. Structure Type – Cadmium Iodide (CdI2) The CdI2 structure can be viewed as a hexagonal close packing (hcp) of iodine, with half of the octahedral holes occupied by cadmium. •There is a weak van der Waals attraction between neighboring iodine layers. •This structure is unstable if the cation-anion bonds have significant ionic character, because of significant anion-anion repulsion. •This structure is seen primarily when the anion is one of the larger halides or chalcogenides. 30 Structure Type – Rutile (TiO2) High refractive index and widely used as white pigments in paints and plastics. -Tetragonal unit cell, but not close packed. Each Ti4+ is coordinated by six O2-. -Each oxygen is surrounded by three planar titaniums, which lie at the corners of an almost equiliateral triangle Structure Type – Corundum (Al2O3) Mineral form is the basis for ruby (Cr) and sapphire (Ti). It is composed of an hcp array of oxygen atoms with two-thirds of the octahedral holes occupied by Al3+. 31 Structure Type – Rhenium Trioxide (ReO3) Also called the aluminum fluoride structure, which is adopted by the fluoride of Al, Sc, Fe, Co, Rh, and Pd, the high temperature form of WO3, and ReO3. -Corner-sharing network of [ReO6] that give a highly symmetrical structure with cubic symmetry. Structure Type – Spinel (MgAl2O4) Spinels have the general formula AB2O4, where generally A is a divalent ion A2+, B is trivalent ion B3+. The structure can be described as being based on a cubic close-packed array of oxide ions, with A2+ ions occupying tetrahedral holes and B3+ ions occupying octahedral holes. A spinel crystal structure containing n AB2O4 structural units has 8n tetrahedral holes and 4n octahedral holes. -1/8th of the tetrahedral holes are occupied by A2+ ions and ½ of the octahedral holes by the B3+ ions. 32 Structure Type – Perovskite (CaTiO3) The structure is named after the mineral CaTiO3. -It has the same octahedral network as the ReO3 structure, with the A ion added into the cavity. -The structure may also be visualized as a ccp array of A and X ions with the B ions occupying the octahedral holes. (Compare with NaCl) -Structures of high-temperature superconductors are based on perovskite. Structure Type – Ilmenite (ABO3) Typically adopted for ABO3 structures where A and B are similar in size and their total charge adds up to +6. -Structure is named after the mineral FeIITiIVO3. -Similar to corundum structure type, where there is a hcp array of oxygen ions, but in ilmenite two different cations are present occupying two-thirds of the octahedral holes. 33 Structures related to close-packed arrangements of anions Formula Cation:anion Coordination Type and number of holes occupied Examples: Cubic close packing Examples: Hexagonal close packing MX 6:6 All octahedral Sodium chloride: NaCl, FeO, MnS, TiC Nickel arsenide: NiAs, FeS, NiS 4:4 Half tetrahedral; every alternate site occupied Zinc blende: ZnS, CuCl, γ-AgI Wurtzite: ZnS, β-AgI 8:4 6:3 All tetrahedral Half octahedral; alternate layers have fully occupied sites Fluorite: CaF2, ThO2, ZrO2, CeO2 Cadmium chloride: CdCl2 None MX3 6:2 One-third octahedral; alterate pairs of layers have two-thirds of the octahedral sites occupied. Bismuth iodide: BiI3, FeCl3, TiCl3, VCl3. M2X3 6:4 Two-thirds octahedral Corundum: αAl2O3, α-Fe2O3, V2O3, Ti2O3, αCr2O3 ABO3 Two-thirds octahedral Ilmenite: Fe2O3 AB2O4 One-eighth tetrahedral and one-half octahedral Olivine: Mg2SiO4 MX2 Cadmium iodide: CdI2 Ionic Radii How does one determine when one atom ‘ends’ and another ‘begins’? -easy for the same atom (e.g. F2), ½ of the distance between the atoms. -what about Na+-Cl- (for example)? High Resolution X-ray diffraction contour map of electron density. -the minimum of electron density along the interionic distances enables accurate determination of the values of the radius for the cation and anion. 34 The effective ionic radii vary depending on coordination number. Size of ions depends on oxidation state. 35 Ionic Radii 36 Trends in sizes of ions 1. The radii of ions within a group increase with atomic number Z. More electrons are present and the outer electrons are further away from the nucleus. 2. In a series of isoelectronic cations (e.g. Na+, Mg2+, Al3+) the radius decreases with increasing positive charge. 3. In a series of isoelectronic anions (e.g. F-, O2-) the radius increases with increasing negative charge. 4. For elements with more than one oxidation state (e.g. Ru4+, Ru5+), the radii decease as the oxidation state increases. 5. As you move from left to right across a row of the periodic table, there is an overall decrease in radius for an similar ions with the same charge. See also the lanthanide contraction. 6. The spin state (high or low spin) affects the ionic radius of transition metals. 7. The radii increase with an increase in coordination number. These trends in the sizes of ions may be explained by consideration of the shielding and effective nuclear charge. Zeff = Z – S Tetrahedral hole Octahedral hole 37 Radius Ratios What are the relative sizes and coordination numbers of the cubic, octahedral, and tetrahedral holes? Size of hole cubic > octahedral Coord. no. 8 6 > tetrahedral 4 If a cation were to occupy one of these holes, it would have the coordination number indicated. -the coordination number is proportional to the size of the hole. How does one calculate the size of a hole? Enables one to predict which size cation would fit into that hole. Cross Section sin(45 ) r r 0.707 2r r 0.414 r Radius ratio for an octahedral hole. 38 Calculate radius ratio for a trigonal hole cos(30 ) r 3 r r 2 30° r 0.155 r r+ rr- Relatively uncommon coordination environment. Use this information to predict which type of hole will be occupied with given ions. Electron-electron repulsion also plays a role in determining the hole the atom occupies. For example, consider the ionic compound NaCl. The 6 coordinate ionic radius (Shannon) of Na+ is 1.16Å and Cl- is 1.67Å. The radius ratio is 1.16/1.67Å = 0.695, therefore falls in the range 0.41 to 0.73 so the Na+ is expected to occupy an octahedral hole. The Cl- is expected to form an A-type lattice – it has a ccp type. The sodium cations occupy the octahedral holes in that lattice. 39 AB Structures Radius ratios, coordination numbers, and coordination environment for both the cations and anions for four representative AB-type ionic lattices. Anions Cations Structure r+/r- Structure C.N. Structure C.N. Sodium chloride (NaCl) 1.16 1.67 ccp (fcc) 6 All octahedral holes 6 Zinc blend (ZnS) 0.88 1.70 ccp (fcc) 4 Half tetrahedral holes 4 Wurtzite (ZnS) 0.88 1.70 hcp 4 Half tetrahedral holes 4 Cesium chloride 1.81 1.67 All cubic holes 8 Simple cubic 8 Compounds with common AB structures Structure Compounds Correlation % Rock Salt alkali halides and hydrides, 58 AgF, AgCl, AgBr, MO (M = Mg, Ca, Sr, Ba, Mn, Fe,Co, Ni, Cd), MS (M = Mg, Ca, Sr, Ba, Mn, Pb), TiC, VC, InP, InAs, SnP, SnAs, NH4I, KOH, KSH, KCN Zinc blende BeX, ZnX, CdX, HgX (X = S, Se, Te), diamond, silicon, germanium, gray tin, SiO2 (cristabolite), BN, BP, SiC, CuX (X = F, Cl, Br, I), XY (X = Al, Ga, In; Y = P, As, Sb) 33 Wurtzite ZnX (X = O, S, Te), CdX (X = S, Se), BeO, MgTe, NH4F, MN (M = Al, Ga, In), AgI 33 Cesium Chloride CsX (X = Cl, Br, I, SH, CN), TlX (X = Cl, Br, I, CN), NH4X (X = Cl, Br,CN) 100 40 (C.N. of A)(no. of A in formula)=(C.N. B)(no. of B in formula) AB2 –type structures Anions Cations Structure r+/r- structure C.N. structure C.N. Fluorite (CaF2) 1.14/1.19 = 0.96 1. 4 1. ½ cubic holes fcc 8 3 ½ of octahedral holes 6 3 Octahedral holes 6 Simple cubic All tetra. 2. 2. Cadmium Iodide (CdI2) 1.09/2.06 = 0.53 hcp Rutile (TiO2) 0.745/1.26 simple tetra. = 0.59 Extended Covalent Arrays Several elements for covalently bonded solids at room temperature, including B, C, Si, Ge, P, As, Se, Te. Unit cell of C (diamond). All C-C bond length are identical (1.54 Å). Covalent C-C bonds are strong and the rigid 3d network of atoms give diamond the hardest substance known and it also has a high melting point. Unit cell of C (graphite). All C-C bond length are identical (1.42 Å). Two dimensional layers of carbon atoms in a hexagonal layer. The distance between layers is 3.40 Å. 41 Covalent Network Crystals A covalent network crystal is composed of atoms or groups of atoms arranged into a crystal lattice, which is held together by an interlocking pair of covalent bonds. Covalent bonds, the sharing of one or more pairs of electrons in a region of overlap between two or more atoms, are directional interactions as opposed to ionic and metallic bonds that are nondirectional. These interactions are directional in nature. Compounds that form covalent network crystals include SiO2, C, Si, BN. Metallic Crystals The structure of metals may be visualized as a lattice of cations held together by a Fermi sea (“of electrons”). The electrons are no longer associated with any particular cation. Valence electrons are delocalized about the lattice of cations. This type of electron movement enables high conductivity typically associated with metals. 42 Ionic Crystals Elemental Ions Na+ Na and Cl and Ionic Bonding NaCl Cl- e- e- e- Picking any Na+, the chloride ion could approach from any direction. Ionic bonds are nondirectional – the electrostatic forces dominate. Many salts form ionic crystals CsCl, CaF2, KNO3, and NH4Cl. Charge-Dipole Interactions Dipole-Dipole Interactions 1/r3 1/r2 London Dispersion Interactions Hydrogen Bonding Interactions 43 Molecular Structures Solid CO2 (dry ice) is a face-centered cubic array of CO2 molecules Type Solid H2O (ice) has several forms depending on P and T Structural Unit Bonding Characteristics Examples Ionic Cations and anions Electrostatic, nondirectional Hard, brittle, high alkali metal m.p.; moderate halides insulators, melts are conducting Extended covalent array Atoms Mainly covalent Strong, hard crystals high m.p. diamond, silica Molecular Molecules Mainly covalent between atoms in a molecule, van der Waals of Hbonding between molecules Soft crystals of low m.p; large coefficient of expansion; insulators ice, organic compounds Metallic Metal atoms Band model m.p. varies, good Fe, Al conductors 44 Silicates – SiO2 SiO2 is polymorphic Quartz cristobalite Silicates – Structural Classification [SiO4]4- (discrete) Olivines, garnets [Si2O7]6- (disilicate) not common, but occur for Sc2Si2O7 [SiO3]2- (chains) pyroxenes [Si4O11]6- (dbl chains) amphiboles (asbestos) [Si4O10]4- ( layers) mica, talc [SiO3]n-2n (rings) beryl (emerald) [SiO4]4-/ [AlO4]5feldspars, zeolites 45 Quasicrystals ordered, but aperiodic Penrose tiling Born-Haber Cycle By accounting for three energies (ionization energy, electron affinity, and lattice energy), we can get a good idea of the energetics of the enthalpy of formation of an ionic solid. 46 Lattice Energy The energy required to completely separate a mole of a solid ionic compound into its gaseous ions; or the energy released when ions (gaseous) form a crystal. Coulombs’s Law The magnitudes of the charges on the ions are Z+ and Z-. (ion pair M+, X-) Z Z e 2 E 4 0 r e2 E 4 0 r e is the electronic charge, 1.6×10-19 C ε0 is the permittivity of vacuum, 8.854×10-12 F m-1 The energy due to the coulombic interactions in a crystal is calculated for a particular structure by summing all the ion-pair interactions, thus producing an infinite series. NaCl √3r0 2r0 √2r0 r0 From a Na+, Six Cl- a distance of r0 EC Twelve Na+ at a distance of √2r0 Eight Cl- at a distance of √3r0 Six Na+ a distance of 2r0 e2 12 8 6 24 (6 ....) 4 0 r 2 3 2 5 or 2 EC e 6 12 8 6 24 ( ....) 4 0 r 1 2 3 4 5 47 EC e2 6 12 8 6 24 ( ....) 4 0 r 1 2 3 4 5 The term (series) inside the brackets is known as the Madelung constant, A. For one mole of NaCl, the energy due to the coulombic interactions is: 2 EC N A Ae 4 0 r NA = Avogadro’s number Madelung constants have been computed for many of the simple ionic structures. Structure Madelung Constant, A Number of ions in formula unit, ν A/ν Coordination Cesium chloride, CsCl 1.763 2 0.882 8:8 Sodium chloride, NaCl 1.748 2 0.874 6:6 Fluorite, CaF2 2.519 3 0.840 8:4 Zinc Blende, ZnS 1.638 2 0.819 4:4 Wurtzite, ZnS 1.641 2 0.821 4:4 Corundum, Al2O3 4.172 5 0.835 6:4 Rutile, TiO2 2.408 3 0.803 6:3 Born exponent Ions are not point charges, but consist of positively charged nuclei surrounded by electron clouds. -repulsion needs to be taken into account at small distances repulsion can be expressed by: ER B rn where B is a constant and n (the Born exponent) is large and also a constant. L EC ER N A AZ Z e 2 B Derivation n 4 0 r r in textbook Ion Type Constant [He] 5 [Ne] 7 [Ar] 9 [Kr] 10 [Xe] 12 L N A AZ Z e 2 1 1 4 0 r n Born-Landé Equation L 1.389 105 AZ Z 1 1 r0 n Calculate average (n), r0 in pm, units of L are kJ/mol e.g. RbCl is 9.5 (Average of 9 and 10) 48 Notice the large dependence on the charge of the ions: L 1.389 105 AZ Z 1 1 r0 n Multiply charged ions tend to have larger lattice energies. It was noted by A.F. Kapustinskii that the Madelung constant divided by the number of ions in one formula unit of the structure (A/ν) was almost constant (0.88 to 0.80). -A general equation can be developed to set up a general lattice energy equation and use the resulting equation to calculate the lattice energy of an unknown structure. L (kJ / mol ) 1.214 105 vZ Z 1 1 r r (in _ pm) n Kapustinskii equations Considering all of the approximations, there is good agreement with values obtained using a Born-Haber cycle, except with large polarizable ions. It is not possible to measure lattice energy directly. Typically a thermochemical cycle is involved, but not all of the data (electron affinities, etc.) is necessarily available. Estimations are useful. -Neil Bartlett used a similar approach to prepare XePtF6. 49